Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 2010RION – ANTIRION BRIDGE PROJECT – CONCRETE DURABILITY TOWARDSCORROSION RISKFrançois Cussigh, Concrete Expert, Vinci Construction France, FranceChristophe Carde, Technical Director, LERM laboratory, FrancePanayotis Papanikolas, PhD, Vice-Chairman and Managing Director, GEFYRA S.A. –Concession Company for the Rion-Antirion Bridge, GreeceAris Stathopoulos - Vlamis, Structural Maintenance Manager, GEFYRA S.A. –Concession Company for the Rion-Antirion Bridge, GreeceABSTRACTThe concrete durability was a major issue for Rion-Antirion Bridge project inGreece due to the adverse environmental site conditions and the contractualrequirement of 120 years service life.The strategy adopted is the corrosion control of embedded steel by reducingthe rate of chloride penetration, which is the great challenge for thedurability, and long service life achievement of concrete structures in marineenvironment. This objective was based on the proper definition of exposurezones, the definition of the appropriate concrete covers and a propercharacterization and evaluation of concrete itself.Specific tests related to the concrete durability parameters were performedsystematically at site laboratory for all mixes used in the project. Acceptancecriteria had been set based on experience. Furthermore, an analysis ofconcrete durability including a service life assessment had been carried outby LERM laboratory. Finally, strict QA/QC procedures were closely followedduring construction to achieve conformity of in-situ quality with that oflaboratory.An additional test schedule is specified in the Inspection and MaintenanceManual during operation in order to evaluate the concrete durability. Theresults obtained during the first two years after the end of constructionconfirm the initial assessments ensuring the overall service life of 120 years.Keywords: Marine Environment, High Performance Concrete, QA/QC Program, ServiceLife Assessment
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20101INTRODUCTIONThe Rion-Antirion Bridge, which was given to traffic in August 2004, consists of the longestmulti-span cable stayed bridge in the world with a continuous deck of 2,252 meters and morethan 600 meters of approach viaducts and further access roads. It is located in the Gulf ofCorinth of Greece and as part of European road network links the Peloponnesus toContinental Greece.The main bridge is a 5-span cable stayed bridge with three spans of 560m and two side onesof 286m. The highest pier/pylon has a total height of 228.5m with the deepest point being63.5m underwater. The main pier foundations measure 90 meters in diameter. The pier baseswere constructed on-site, before they were floated into position in the Gulf, and lowered ontothe seabed using water as ballast. The four main pylons were built in concrete using climbingshutters, and they reach 164 meters above sea level.Fig. 1 Rion-Antirion Bridge ProjectA major issue was the long-term performance of concrete structures in a marine environmentsince the contractual specifications were requiring a service life of 120 years.A specific strategy for the long-term concrete durability was adopted and various tests wereperformed to validate the specifications. Additionally, a QA/QC program was strictlyfollowed for concrete production/construction to achieve a homogeneous structure fulfillingthe specifications. Further to that, the Supervisor Engineer instructed several tests at specificlocations.For the follow up of concrete durability a program has been set, which defines specific teststo be performed during the operational period on regular basis in order to measure thechlorides penetration, to determine the chlorides diffusivity and assess the overall service lifeof the structure.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20102CONCRETE DURABILITY STRATEGYIn order to achieve the 120 years of service life, it was very important to characterize andevaluate properly the concretes ability to protect the embedded steel from corrosion.The three major degradation risks on reinforced concrete were the chemical attack byseawater, the corrosion induced by chlorides, the corrosion induced by CO2.The strategy chosen to protect the steel relied mainly on concrete durability, which includes aproper definition of exposure zones, the definition of appropriate concrete covers, and aproper characterization and evaluation of concrete itself.EXPOSURE ZONESThe structure was divided into the following parts:• Pile Viaducts Foundations (bored or composite)• Substructure externally exposed below MSL (Mean Sea Level) +10m divided into:o Immersed zone below MSL –5mo Tidal & splash zone between MSL –5m & MSL +10m• Substructure externally exposed above MSL +10m• Substructure overland• Bridge and Viaducts SuperstructureThe most exposed zones in terms of corrosion risk are the structures externally exposedbelow MSL + 10m.The immersed zone (below MSL -5.0m) is much less critical than the splash and tidal zone(between MSL -5.0m and MSL +10.0m), due to the lack of oxygen in this area.DEFINITION OF COVERSThe different covers of the structure have been defined, with the assistance of concretedurability experts, in accordance to the durability criteria selected. As a result, higher coverthan contractually required has been selected (for the same exposure zone), especially incritical zones. Table 1 summarizes the covers selected for the Rion-Antirion Bridge andapplied throughout construction for the different exposure zones. A comparison with thecontractual specifications shows that in the ‘immersed zone’ and ‘tidal and splash zone’ thecover has been increased by 20% and 13%, respectively.Table 1 Covers in relation to exposure zone (values are in mm)Exposure SituationContractualSpecifications (mm)MinimumNominal Cover(mm)Viaducts Pile Foundations (bored or composite) - 100Immersed zone (below MSL –5m) 50 60Tidal & Splash (MSL –5m to MSL +10m) 75 85Substructure externally exposed above MSL +10m 50 50Substructure over land 45 50
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20103Deck lower free surface 40 40Bridge & ViaductSuperstructure Deck upper surface 30 30CONCRETE SPECIFICATIONS TOWARDS DURABILITYConcrete specifications refer mainly to the selection of the constituents, the content ofcement and the Water/Cement Ratio, according to the exposure situation of each part of thestructure, with special specifications for marine environment.Selection of constituentsThe concrete constituents have been selected by mix design experts in order to ensure therequired quality of the concrete in situ. The stability of concrete constituents, their propertiesand their proportions were major factors to guarantee a constant and uniform concreteproduction. They were established after a long series of trials.CementMost of concrete mixes have been mixed with cement type CEM III 42.5 PM ES with slagcontent higher than 60%. A local supplier had specially produced this type of cementaccording to the projects requirements. It had a low heat of hydration and was adequate formarine exposure environments. The other types used are shown below in figure 2.AggregatesThe aggregates used were crushed limestone stone and came from the quarry of a localsupplier. It was divided in three fractions: coarse1 10/20, coarse2 4/10 and sand 0/4. Theaggregate supplier had to supply specific sand, in which the fines content was regulatedaround 9%. Siliceous sand could not been used because of alkali-silica reaction risks.AdmixturesThe admixtures had been chosen among numerous products. For instance, Optima 100,Glenium 27 and Rheobuilt T3 had been selected for their technical characteristics.Figure 2 presents the concrete class with the cement type for the main piers and pylonsstructures.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20104Fig. 2 Main piers and pylonsThe types of cement used had the following characteristics.• CEM III is blast furnace slag cement CEM III/A 42.5 with 60% to 64% of slag.• CEM II is CEM II/B-M (W-P-LL) 32.5 N.• CEM I is CEM I 52.5.All concrete mixes had a maximum W/C ratio of 0.40.VALIDATION OF CONCRETE SPECIFICATIONSIn order to validate the concrete quality and durability requirements a strategy has beendeveloped throughout the construction.This strategy included • a series of laboratory tests,• QA/QC procedures of concrete construction,• and tests made in-situ.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20105LABORATORY TESTSAll the cores and samples tested were coming from concrete cast, which was made forlaboratory purposes at the Site Batching Plant under the same conditions as those of regularproduction. Certain acceptance criteria, which were based on experience, had been chosenfor the verification of the test results.Rapid Chloride Penetration Test and Water Penetration TestThe RCPT1result (Rapid Chloride Penetration Test), combined with the WDP2(WaterPenetration Test), were used as the main durability indicator. These two tests have beenperformed systematically at the KG site laboratory on all Conformity Trials for each differentmix defined for the structure.The respect of fresh concrete parameters within acceptable tolerances defined in Trial MixReports, guaranteed results on hardened concrete (strength and durability characteristics)equivalent to the ones obtained during those conformity trials.The acceptance criteria for those tests have been chosen so that:• WDP ≤ 20mm• RCPT at 90 days ≤ 1000C (Coulomb) in the splash zone≤ 2000C for substructures≤ 4000C for piles-foundations and Bridge & Viaduct superstructureTable 2 RCPT results of concrete mixes used on siteMixNoClass ofConcreteUse of Mix Exposure ClassType and quantity ofCementDmax(mm)W/CRatioRCPT Resultsmin-max (C)420 C45/55 Pier BaseSubstructurebelow MSL +10CEM III 400 kg/m320 0.40 480-1050425428C45/55ConeOctagonImmersed zonebelow MSL -5CEM III 420 kg/m3 20 0.39 220-600432 C45/55Raft &Walls infootingImmersed zonebelow MSL –5CEM III 450 kg/m310 0.40 430-880520 C50/60 Pylon BaseSubstructureabove MSL +10CEM III 420 kg/m320 0.37 200-360610 C60/75Pier shaftslabSplash zoneMSL –5/+10CEM III 490 kg/m320 0.33 220-390620 C60/75 Pylon legsSuperstructure ofMain BridgeCEM III 327 kg/m3CEM I 163 kg/m3 20 0.33 270-575612 C60/75Deck onshoreSuperstructure ofMain BridgeCEM III 490 kg/m320 0.33 320-370670 C60/75Deck offshoreSuperstructure ofMain BridgeCEM I 450 kg/m320 0.33 1300-2100
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20106Determination of chloride binding capacityA specialized external laboratory had measured the chloride binding capacity on samples castin the site laboratory. These samples were made of concrete mixes, which were intended tobe used in the zone below MSL +10m (immersed and splash & tidal zone).Fig. 3 Interaction isotherms of chloride (bound chlorides versus total chlorides)From the results shown on Figure 3, the capacity of the chloride fixation of the binder is veryhigh, approximately 50% of the total chlorides (0 – 2 % range). The binding capacity isapproximately the same for the two different mixes of concrete used.Measurement of Oxygen PermeabilityMeasurements of Oxygen Permeability (AFPC-AFREM method) have been performed oncores taken from walls cast with 425 and 430 formula of C45/55, cured 3 days with water,and then installed in splash and tidal zone on site. The scope was to simulate concrete cast insitu (cone, pier shaft), and expose in splash and tidal zone at a very early age (probably theworst situation).The oxygen permeability has been measured to be < 1x10-17m2at 28 days. This indicates theconcrete’s ability to prevent air and water ingress (necessary agents for steel corrosion).Determination of chloride diffusion coefficientMeasurements of chloride diffusion coefficient (TANG LUPINGs method)3have beenperformed on cores taken from the same walls mentioned above by an external specializedlaboratory.The chloride diffusivity has been measured to be < 1x10-12m2/s at 28 days and < 5x10-13m2/safter 4 months. The results correspond to concrete of high compactness.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20107The results of chloride diffusion coefficient obtained at different ages on concrete blocks,combined with the chloride binding capacity of the cement paste have been used as inputdata in a finite element model used to simulate the service life of the bridge.The variation of the diffusion coefficient with respect to time is the most important parameterfor the simulation. The equation used to describe its evolution corresponds to the generalequations found in the literature 4and used for the durability prediction of the Vasco DaGama Bridge:D = a t-α(1)where D: Chlorides diffusion coefficient in m2/s.t: time in month.a and α : correspond respectively to the reference value of the chlorides diffusioncoefficient at t0, and to the aging factor. These terms are experimentallydetermined with the measurements of the chlorides diffusion coefficient atseveral age of the concrete.The values initially taken were a=1x10-12and α=0.4297, based on experimental data fromVasco Da Gama Bridge.The software used was already applied for the concrete durability of Vasco da Gama Bridge,which is located in the Tagus bay in Lisbon [Houdusse, Hornain and Martinet, 2000] 5. Thissoftware includes a mathematical model, which describes the transport equation of achemical species, and a finite element model, which corresponds to the spatial discretizationof the mathematical model.The numerical simulations permit a variation of concrete characteristics with space and time.Furthermore, the variation of the diffusion coefficient with respect to time is the one of themost important parameter for the simulation.Capillary and porosity tests – ResistivityIn order to validate the high performance of the concrete especially used in immersed andsplash zones after the recommendation of the concrete expert, Odd E. Gjørv6(NorwegianUniversity of Science and Technology) some further tests have been performed. The testsperformed at KG site laboratory are the following:• Capillary and porosity tests• Resistivity measurements (use of RCPT test)The main results are presented in the following table.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20108Table 3 Additional KG laboratory testsQA/QC PROCEDURES FOR CONCRETE PRODUCTION AND CONSTRUCTIONIn order to proceed with the concrete production in daily basis, the moisture content of theaggregates, the consistency (slump and flow) and the temperature of the concrete werechecked. In order to begin the concrete production, the workability values had to agree withthe conformity values and the concrete temperature had to be satisfactory for that seasonalperiod.In case the values were not in agreement with the conformity values, corrective action wastaken. That included adjusting the water quantity per cubic meter (±5 liters) and theMixNoClass ofConcreteUse of Mix Exposure Class Type ofCementW/CRatioResistivitymin-max(Ohm.m))CapillaryNumber Kmin-max(kg/m2/s-0,5)CapillaryResistanceNumber Mmin-max(s/m2)SuctionPorosity(%)406420C45/55 Pier BaseRafts andPrecast slabsSubstructureexternally exposedbelow MSL +10(immersed zonebelow MSL –5)Cem III400kg/m30.4 360 –7501.0x10-21.4 x 10-27.5 x 1062.6 x 1079.313.0423429439C45/55 Rafts, Walls,Footing Topslab in DryDockAntirion &Rion ViaductSubstructure inSplash zoneSubstructureexternally exposedbelow MSL +10(immersed zonebelow MSL –5) andSplash Zone (MSL-5 to MSL +10)Cem III400kg/m30.4 350 –6409.0 x 10-31.3 x 10-21.2 x 1072.0 x 1078.511.8425428438C45/55 Cone at WetDockOctagon InSituPier Head InSituRion Viaductbored piles inSplash zoneImmersed zonebelow MSL –5Splash & tidal zone(MSL –5 to MSL+10)Cem III420kg/m3< 0.4 380 –6809.0 x 10-31.2 x 10-28.0 x 1061.7 x 1078.110.6446 C45/55 Mass Concretein Dry Dockand In situ(Pier Head)Immersed zone(below MSL –5) &Substructureexternally exposedabove MSL +10Cem III450kg/m30.39 470 –6001.3 x 10-22.0 x 10-21.3 x 1071.5 x 10711.212.5
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 20109admixture quantity per cubic meter (±0.5kg). The proportion of hot/cold water was adjustedin order to obtain the required concrete temperature.Each 100m3or per construction part (in case the quantity was less), samples were taken toverify the compressive strength. Extra samples were taken for information on early agedepending on the constructions needs, such as stripping of the formwork, pre-stressing etc.During the concrete construction, good workmanship was well prepared with Work MethodStatements and controlled under Inspection and Test Schedules. They were used to defineprecisely important factors for each part of the structure such as the specific mix design, thecuring process, the minimum actual cover, etc. The curing of the concrete on site, forinstance, was carefully followed up, especially in critical zones.Finally, it is also important to notice that cover was also carefully controlled on site beforethe casting of structure parts and also after formwork removal, via a cover meter on randomareas, and wherever difficulties or problems have been met before and/or during casting.From a design point of view two values of concrete cover were specified; the actualminimum value (value assumed in the concrete durability design & follow-up) and thenominal minimum cover (used during construction) which was 5-10mm larger in order toaccount for construction tolerances. This provided an additional security level that theminimum cover was obtained during construction.Statistical evaluation of concrete production resultsOn Table 4 the average value and standard deviation of 28 days compressive strengths as pertotal production and as per concrete class is shown.Table 4 Average strengths and standard deviations by concrete classConcreteClassMix numberAmount ofcement(kg/m3)Average strength(MPa)StandardDeviation(MPa)C40/50 416/418 450 74.4 3.7406 400 76.6 4.8425/426/428/429 420 68.6 4.8C45/55420 400 69.9 4.9520 420 75.0 3.2C50/60446 450 75.0 4.2610 490 82.0 5.0612 490 79.8 2.6620 490 80.6 2.8C60/75670 490 80.5 2.0
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 201010IN-SITU TESTSRCPT measurementsIn order to verify the adequacy of laboratory concrete with in-situ one, some cores wereextracted from parts of the structure, which were appointed by the Supervision Engineer andappeared that they were not perfectly made or cured. The RCPT values of those cores arepresented in table 5.Table 5 RCPT resultsMixNumberDate of casting Exposure Zone RCPT Results onproduction samples(Coulomb)RCPT Laboratory resultson the same formula(Coulomb)406 7/12/99 Immersed Zone(below MSL - 5.0m)697 480 - 1050429 11/04/0016/03/0028/03/00Immersed Zone(below MSL - 5.0m)670-763-786733635-590650 - 1040446 16/07/01 Splash Zone (betweenMSL - 5.0m and MSL+10.0m)351-390-341 450 - 500The results show a perfect compliance of the production concrete with the laboratory results.Validation of uniformity of In-Situ Concrete QualityIn order to validate the uniformity of the in-situ concrete, non-destructive tests wereperformed on each pier, and specifically at the first lift of the pier shaft on the internal side.Two methods were used to get precision in the results: sclerometry and ultrasonic. Thesclerometer measures the hardness of the concrete surface, whereas the ultrasonicauscultation relates with the homogeneity and the cracking of the materials.The objective was to determine the classification of different compacity areas (low, medium,high). From the results, the quality of compacity was defined, in order to select the zonesfrom which samples could be extracted.From each selected zone, six cores were extracted by site laboratory so as to be submitted tochloride diffusion coefficient measurements (external laboratory) and RCPT tests (sitelaboratory).The synthesis of the measurements is presented in Table 6.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 201011Table 6 In situ chloride diffusion coefficient (D) and RCPT resultsPierConstructionage (month)Compacity zoneMean value of D(1x10-12m2/s)Standarddeviation of 3cores(1x10-12m2/s)Standard deviation ofthe measurements(1x10-12m2/s)Min-maxvalue(1x10-12m2/s)medium 0.53 0.21M1 24low 0.74 0.41medium 0.22 0.05M2 21low 0.26 0.11medium 0.38 0.07M3 36low 0.30 0.17medium 0.32 0.20M4 33low 0.71 0.290.27 0.22-0.98PierConstructionage (month)Compacity zoneMean value ofRCPTmeasurements (C)Standarddeviationbetween the 3cores (C)Standard deviation ofthe measurements (C)Min-maxvalue (C)medium 269 12M1 24low 292 32medium 331 38M2 21low 221 4medium 260 35M3 36low 289 51medium 242 69M4 33low 278 18441 221-365SERVICE LIFE ASSESSMENTIn pursuance of assuring its long-term performance, a follow-up on concrete durability isessential. Following the philosophy of validating the durability requirements, tests need to bemade after the end of the construction.It is preferable that destructive tests are avoided in-situ for obvious reasons. As aconsequence, a sacrificial reinforced concrete wall element was built on P2 pile cap (off-shore pier of Rion approach viaduct) in summer 2004 so as to provide samples fordestructive tests.LONG-TERM PERFORMANCE APPROACHTestsConsidering the fact that the chloride penetration is the most important factor to evaluate thecorrosion risk to the embedded steel, it is necessary to determine its evolution through timeso as to establish the service life of the bridge.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 201012In that scope, tests are carried out with respect to chloride diffusivity and chloride bindingcapacity by an external specialized laboratory. The results of these tests give the data to anumerical simulation of the expected service life.The tests performed are:• Determination of the chloride diffusion coefficient according to TANG LUPING method.• Measurement of total and free chlorides contents as a function of the depth (from the faceof the concrete to 80mm).Numerical simulationThe objectives of the numerical simulation are to predict the lifetime evolution of thechlorides penetration and to compare it with the concrete cover and the critical chloridesthreshold. The simulations are made for the current term and for a 120 year duration, whichcorresponds to the bridge’s service life.A major parameter for the model is the evolution law of the Chlorides diffusion coefficient.Evolution lawAs it was already mentioned above, the variation of the diffusion coefficient with respect totime is very important for the simulation.Initially, the law used for the numerical simulations corresponds to the one established forthe concrete in the Vasco De Gama Bridge Project (D=1x10-12x t-0.4297). This law was usedbecause the first values show a good correlation and the concrete used for both bridges issimilar.The law currently considered in the updated numerical simulations (after the additionalmeasurement results acquired from in-situ tests) is as follows:D = 1x10-12.t-0.2868(2)
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 201013Fig. 4 Evolution of the diffusion coefficient with timeAt the simulation, this law is applied during the first 10 years. After 10 years, the Chloridesdiffusion coefficient is considered as a constant value. The measurements of the diffusioncoefficient that will follow are meant to confirm the law used.SACRIFICIAL WALLThroughout construction, one sacrificial reinforced in-situ concrete wall element was cast atthe same time as the actual structure under the same circumstances (formula, personnel,conditions). The 1m high 5m long and 0.5m wide element was poured on P2 pile cap of theRion approach viaduct, with Ø20mm reinforcement every 200mm and a minimum actualcover of 50mm on both sides.This wall allows measuring the real chloride ingress at different ages, even after theconstruction period. Samples are taken periodically to carry out tests as it was explainedabove. The position of the samples is pre-marked, in order to avoid cutting the reinforcement.COMPARISON OF REAL CHLORIDE INGRESS AND SIMULATED VALUESSamples from the sacrificial wall have already been studied at the ages of 3 months (in2004), 11 months (in 2005) and 24 months (in 2006). The total chlorides profiles measuredare given in Figure 5 below. These results show a significant increase of chlorides contentonly in the first 10 mm from the surface.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 201014Fig. 5 Evolution of total chlorides contents with timeThe numerical simulations have been made with the new law of diffusion coefficientevolution, and with a limit condition about 3.5%/kg of cement based on experimental results.The results of numerical simulations have been obtained at the ages of 24 months and 120years (service life).The results obtained show that the concrete from reinforced wall complies with the durabilityrequirement of 120 years with regards to the corrosion risk because the free chlorides contentis under the threshold of 0.4% (of cement). The threshold is determined based on EN 206-1 7,where it refers to concrete class XS3 for steel reinforced concrete and applies for the splashand tidal zone. Actually, in national French appendix (NF EN 206-1) there is also theclassification for steel reinforced concrete with CEM III, which applies for the Rion-AntirionBridge and the threshold is 0.65%.
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 201015Fig. 6 Simulation for 2 years old concrete compared to the chlorides contents measured(Solid line) and simulation at 120 years (dashed line) for a limit condition equal to 3.5%CONCLUSIONSConcrete results obtained at laboratory and on site show a very good ability of Rion-AntirionBridge concrete to protect the embedded steel from corrosion, and guarantee the achievementof a 120 years service life. A follow up of in situ concrete with same testing has been carriedout 3 times during the first two years of operation and it will be continued over the next yearsto confirm its quality towards durability requirements and obtain more results allowing asafer assessment of service life.REFERENCES1. ASTM C 1202 Standard Test Method for Electrical Indication of Concretes Ability toResist Chloride Ion Penetration2. ISO 7031 Concrete hardened; determination of the depth of penetration of water underpressure3. NT Build 492: CTH Rapid Test4. Conception des bétons pour une durée de vie donnée des ouvragesGuide pour la mise en œuvre d’une approche performantielle et prédictive sur la based’indicateur de durabilité. Documents scientifiques et techniques de l’AFGC (AssociationFrançaise de Génie-Civil) - Juillet 2004
Cussigh, Carde, Papanikolas, Stathopoulos-Vlamis 3rdfib International Congress – 2010165. Houdusse O., Hornain H. and Martinet G. (2000) Prediction of Long-Term Durability ofVasco Da Gama Bridge in Lisbon. Fifth International Conference of CANMET/ACI.Barcelona. 1037.6. Odd E. Gjørv and Rui Miguel Ferreira (2002) Rion Antirion Bridge Report. Confidentialreport7. EN 206-1: Concrete – Part 1: Specification, performance, production and conformityAKNOWLEDGEMENTS1. LERM: External specialized laboratory.2. MacBeton Hellas: Supplier for concrete admixtures, such as Glenium, Pozzolith,Rheobuilt, etc.3. Chryso: Supplier for concrete admixtures, such as Optima 100.4. TITAN: Cement supplier.5. Lafarge Araxos: Aggregates supplier.